LMucko/crystallography-open-database huggingface dataset:
Crystal structure and physical properties of new Ca2TGe3 (T = Pd and Pt) germanides
Klimczuk, T.; Xie, Weiwei; Winiarski, M.J.; Koziol, R.; Litzbarski, L.S.; Luo, Huixia; Cava, R.J.; Journal of Solid State Chemistry 243 (2016) 95–100; doi:10.1016/j.jssc.2016.07.029

data_1543916
_publ_section_title
;
 Crystal structure and physical properties of new Ca2TGe3 (T = Pd and Pt)
 germanides
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              95
_journal_page_last               100
_journal_paper_doi               10.1016/j.jssc.2016.07.029
_journal_volume                  243
_journal_year                    2016
_chemical_formula_structural     'Ca2 Pd Ge3'
_chemical_formula_sum            'Ca2 Ge3 Pd'
_space_group_IT_number           191
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   8.4921(1)
_cell_length_b                   8.4921(1)
_cell_length_c                   4.1922(1)
_cell_volume                     261.820(8)
_refine_ls_R_factor_all          0.0693
_cod_data_source_file            Ca2PdGe3_COD.cif
_cod_data_source_block           Ca2PdGe3
_cod_depositor_comments          'Corrected wrong journal name.'
_cod_original_cell_volume        262
_cod_database_code               1543916
Crystal structure and physical properties of new Ca2TGe3 (T = Pd and Pt) germanides
Klimczuk, T.; Xie, Weiwei; Winiarski, M.J.; Koziol, R.; Litzbarski, L.S.; Luo, Huixia; Cava, R.J.; Journal of Solid State Chemistry 243 (2016) 95–100; doi:10.1016/j.jssc.2016.07.029

data_1543917
_publ_section_title
;
 Crystal structure and physical properties of new Ca2TGe3 (T = Pd and Pt)
 germanides
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              95
_journal_page_last               100
_journal_paper_doi               10.1016/j.jssc.2016.07.029
_journal_volume                  243
_journal_year                    2016
_chemical_formula_structural     'Ca2 Pt Ge3'
_chemical_formula_sum            'Ca2 Ge3 Pt'
_space_group_IT_number           191
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   8.4520(1)
_cell_length_b                   8.4520(1)
_cell_length_c                   4.2188(1)
_cell_volume                     260.999(8)
_refine_ls_R_factor_all          0.1180
_cod_data_source_file            Ca2PtGe3_COD.cif
_cod_data_source_block           Ca2PtGe3
_cod_depositor_comments          'Correction of wrong journal name.'
_cod_original_cell_volume        261
_cod_database_code               1543917
Triple molybdate scheelite-type upconversion phosphor NaCaLa(MoO4)3:Er(3+)/Yb(3+): structural and spectroscopic properties.
Lim, Chang Sung; Aleksandrovsky, Aleksandr S.; Molokeev, Maxim S.; Oreshonkov, Aleksandr S.; Ikonnikov, Denis A.; Atuchin, Victor V.; Dalton transactions (Cambridge, England : 2003) 45 (2016) 15541–15551; doi:10.1039/c6dt02378a

data_7040528
_publ_section_title
;
 Triple molybdate scheelite-type upconversion phosphor
 NaCaLa(MoO4)3:Er(3+)/Yb(3+): structural and spectroscopic properties.
;
_journal_issue                   39
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              15541
_journal_page_last               15551
_journal_paper_doi               10.1039/c6dt02378a
_journal_volume                  45
_journal_year                    2016
_chemical_formula_moiety         'Er0.07 La0.67 Mo4 O16 Yb0.60, 1.333(Ca Na)'
_chemical_formula_sum            'Ca1.33 Er0.07 La0.67 Mo4 Na1.33 O16 Yb0.6'
_chemical_formula_weight         931.47
_space_group_IT_number           88
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4ad'
_symmetry_space_group_name_H-M   'I 41/a :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   5.242071(96)
_cell_length_b                   5.242071(96)
_cell_length_c                   11.46775(23)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    300
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     315.126(10)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    63.714
_exptl_crystal_density_diffrn    4.90808
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 4 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        9.970
_pd_proc_ls_prof_wR_expected     13.493
_pd_proc_ls_prof_wR_factor       15.061
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.116
_refine_ls_R_I_factor            1.65
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            c6dt02378a1.cif
_cod_data_source_block           a
_cod_depositor_comments
;Adding full bibliography for 7040528--7040531.cif.

 Adding full bibliography for 7040528--7040531.cif.
;
_cod_original_cell_volume        315.126(13)
_cod_original_sg_symbol_Hall
;
-I 4ad
;
_cod_original_sg_symbol_H-M      I41/a
_cod_original_formula_sum
;
Ca1.33 Er0.07 La0.67 Mo4 Na1.33 O16 Yb0.60
;
_cod_database_code               7040528
Triple molybdate scheelite-type upconversion phosphor NaCaLa(MoO4)3:Er(3+)/Yb(3+): structural and spectroscopic properties.
Lim, Chang Sung; Aleksandrovsky, Aleksandr S.; Molokeev, Maxim S.; Oreshonkov, Aleksandr S.; Ikonnikov, Denis A.; Atuchin, Victor V.; Dalton transactions (Cambridge, England : 2003) 45 (2016) 15541–15551; doi:10.1039/c6dt02378a

data_7040529
_publ_section_title
;
 Triple molybdate scheelite-type upconversion phosphor
 NaCaLa(MoO4)3:Er(3+)/Yb(3+): structural and spectroscopic properties.
;
_journal_issue                   39
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              15541
_journal_page_last               15551
_journal_paper_doi               10.1039/c6dt02378a
_journal_volume                  45
_journal_year                    2016
_chemical_formula_moiety         'Ca1.33 La1.33 Mo4 Na1.33 O16'
_chemical_formula_sum            'Ca1.33 La1.33 Mo4 Na1.33 O16'
_chemical_formula_weight         909.04
_space_group_IT_number           88
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4ad'
_symmetry_space_group_name_H-M   'I 41/a :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   5.29916(13)
_cell_length_b                   5.29916(13)
_cell_length_c                   11.62227(28)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    300
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     326.366(14)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    69.036
_exptl_crystal_density_diffrn    4.625223
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 4 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        13.392
_pd_proc_ls_prof_wR_expected     16.222
_pd_proc_ls_prof_wR_factor       19.463
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.200
_refine_ls_R_I_factor            5.29
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            c6dt02378a4.cif
_cod_data_source_block           a
_cod_depositor_comments
;Adding full bibliography for 7040528--7040531.cif.

 Adding full bibliography for 7040528--7040531.cif.
;
_cod_original_cell_volume        326.366(17)
_cod_original_sg_symbol_Hall
;
-I 4ad
;
_cod_original_sg_symbol_H-M      I41/a
_cod_original_formula_sum
;
Ca1.33 La1.33 Mo4 Na1.33 O16
;
_cod_database_code               7040529
Triple molybdate scheelite-type upconversion phosphor NaCaLa(MoO4)3:Er(3+)/Yb(3+): structural and spectroscopic properties.
Lim, Chang Sung; Aleksandrovsky, Aleksandr S.; Molokeev, Maxim S.; Oreshonkov, Aleksandr S.; Ikonnikov, Denis A.; Atuchin, Victor V.; Dalton transactions (Cambridge, England : 2003) 45 (2016) 15541–15551; doi:10.1039/c6dt02378a

data_7040530
_publ_section_title
;
 Triple molybdate scheelite-type upconversion phosphor
 NaCaLa(MoO4)3:Er(3+)/Yb(3+): structural and spectroscopic properties.
;
_journal_issue                   39
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              15541
_journal_page_last               15551
_journal_paper_doi               10.1039/c6dt02378a
_journal_volume                  45
_journal_year                    2016
_chemical_formula_moiety         'Er0.13 La0.93 Mo4 O16 Yb0.27, 1.333(Ca Na)'
_chemical_formula_sum            'Ca1.33 Er0.13 La0.93 Mo4 Na1.33 O16 Yb0.27'
_chemical_formula_weight         921.92
_space_group_IT_number           88
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4ad'
_symmetry_space_group_name_H-M   'I 41/a :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   5.26749(13)
_cell_length_b                   5.26749(13)
_cell_length_c                   11.53772(32)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    300
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     320.131(14)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    65.247
_exptl_crystal_density_diffrn    4.782144
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 4 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        10.313
_pd_proc_ls_prof_wR_expected     13.612
_pd_proc_ls_prof_wR_factor       15.649
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.150
_refine_ls_R_I_factor            2.09
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            c6dt02378a2.cif
_cod_data_source_block           a
_cod_depositor_comments
;Adding full bibliography for 7040528--7040531.cif.

 Adding full bibliography for 7040528--7040531.cif.
;
_cod_original_cell_volume        320.130(19)
_cod_original_sg_symbol_Hall
;
-I 4ad
;
_cod_original_sg_symbol_H-M      I41/a
_cod_original_formula_sum
;
Ca1.33 Er0.13 La0.93 Mo4 Na1.33 O16 Yb0.27
;
_cod_database_code               7040530
Triple molybdate scheelite-type upconversion phosphor NaCaLa(MoO4)3:Er(3+)/Yb(3+): structural and spectroscopic properties.
Lim, Chang Sung; Aleksandrovsky, Aleksandr S.; Molokeev, Maxim S.; Oreshonkov, Aleksandr S.; Ikonnikov, Denis A.; Atuchin, Victor V.; Dalton transactions (Cambridge, England : 2003) 45 (2016) 15541–15551; doi:10.1039/c6dt02378a

data_7040531
_publ_section_title
;
 Triple molybdate scheelite-type upconversion phosphor
 NaCaLa(MoO4)3:Er(3+)/Yb(3+): structural and spectroscopic properties.
;
_journal_issue                   39
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              15541
_journal_page_last               15551
_journal_paper_doi               10.1039/c6dt02378a
_journal_volume                  45
_journal_year                    2016
_chemical_formula_moiety         'Er0.27 La1.07 Mo4 O16, 1.333(Ca Na)'
_chemical_formula_sum            'Ca1.33 Er0.27 La1.07 Mo4 Na1.33 O16'
_chemical_formula_weight         916.66
_space_group_IT_number           88
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4ad'
_symmetry_space_group_name_H-M   'I 41/a :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   5.28062(15)
_cell_length_b                   5.28062(15)
_cell_length_c                   11.57258(34)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    300
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     322.701(16)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    66.187
_exptl_crystal_density_diffrn    4.716673
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 4 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        11.298
_pd_proc_ls_prof_wR_expected     14.872
_pd_proc_ls_prof_wR_factor       16.751
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.126
_refine_ls_R_I_factor            3.15
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            c6dt02378a3.cif
_cod_data_source_block           a
_cod_depositor_comments
;Adding full bibliography for 7040528--7040531.cif.

 Adding full bibliography for 7040528--7040531.cif.
;
_cod_original_cell_volume        322.700(20)
_cod_original_sg_symbol_Hall
;
-I 4ad
;
_cod_original_sg_symbol_H-M      I41/a
_cod_original_formula_sum
;
Ca1.33 Er0.27 La1.07 Mo4 Na1.33 O16
;
_cod_database_code               7040531
Structure evolution and photoluminescence of Lu3(Al,Mg)2(Al,Si)3O12:Ce3+ phosphors: New yellow-color converter for blue LED-driven solid state lighting
Haipeng Ji; Le Wang; Maxim Molokeev; Naoto Hirosaki; Rong-Jun Xie; Zhaohui Huang; Zhiguo Xia; Otmar Melvin ten Kate; Lihong Liu; Victor V. Atuchin; Journal of Materials Chemistry C 4 (2016) 6855–6863; doi:10.1039/c6tc00966b

data_7226445
_publ_section_title
;
 Structure evolution and photoluminescence of Lu3(Al,Mg)2(Al,Si)3O12:Ce3+
 phosphors: New yellow-color converter for blue LED-driven solid state
 lighting
;
_journal_issue                   0
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              6855
_journal_page_last               6863
_journal_paper_doi               10.1039/c6tc00966b
_journal_volume                  4
_journal_year                    2016
_chemical_formula_moiety         'Al40 Ce0.24 Lu23.76 O96'
_chemical_formula_sum            'Al40 Ce0.24 Lu23.76 O96'
_chemical_formula_weight         6806.12
_space_group_IT_number           230
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I a -3 d'
_audit_update_record
;
2015-12-03 # Formatted by publCIF
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   11.913627(45)
_cell_length_b                   11.913627(45)
_cell_length_c                   11.913627(45)
_cell_measurement_reflns_used    109
_cell_measurement_temperature    300
_cell_measurement_theta_max      60
_cell_measurement_theta_min      7.5
_cell_volume                     1690.955(11)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    71.424
_exptl_crystal_density_diffrn    6.683636
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        120
_pd_meas_2theta_range_min        15
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
no preferred orientation
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        7.831
_pd_proc_ls_prof_wR_expected     4.676
_pd_proc_ls_prof_wR_factor       10.831
_pd_proc_number_of_points        5250
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   2.316
_refine_ls_R_I_factor            3.19
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            Lu2p97Ce0p03Al5O12.cif
_cod_data_source_block           a
_cod_original_cell_volume        1690.955(19)
_cod_original_sg_symbol_Hall
;
-I 4bd 2c 3
;
_cod_original_sg_symbol_H-M      Ia-3d
_cod_original_formula_sum
;
Al40 Ce0.24 Lu23.76 O96
;
_cod_database_code               7226445
_cod_database_fobs_code          7226445
Structure evolution and photoluminescence of Lu3(Al,Mg)2(Al,Si)3O12:Ce3+ phosphors: New yellow-color converter for blue LED-driven solid state lighting
Haipeng Ji; Le Wang; Maxim Molokeev; Naoto Hirosaki; Rong-Jun Xie; Zhaohui Huang; Zhiguo Xia; Otmar Melvin ten Kate; Lihong Liu; Victor V. Atuchin; Journal of Materials Chemistry C 4 (2016) 6855–6863; doi:10.1039/c6tc00966b

data_7226446
_publ_section_title
;
 Structure evolution and photoluminescence of Lu3(Al,Mg)2(Al,Si)3O12:Ce3+
 phosphors: New yellow-color converter for blue LED-driven solid state
 lighting
;
_journal_issue                   0
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              6855
_journal_page_last               6863
_journal_paper_doi               10.1039/c6tc00966b
_journal_volume                  4
_journal_year                    2016
_chemical_formula_moiety         'Al32 Ce0.24 Lu23.76 Mg4 O96 Si4'
_chemical_formula_sum            'Al32 Ce0.24 Lu23.76 Mg4 O96 Si4'
_chemical_formula_weight         6799.88
_space_group_IT_number           230
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I a -3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   11.938448(35)
_cell_length_b                   11.938448(35)
_cell_length_c                   11.938448(35)
_cell_measurement_reflns_used    109
_cell_measurement_temperature    300
_cell_measurement_theta_max      60
_cell_measurement_theta_min      7.5
_cell_volume                     1701.546(9)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    71.013
_exptl_crystal_density_diffrn    6.635894
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        120
_pd_meas_2theta_range_min        15
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
no preferred orientation
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.431
_pd_proc_ls_prof_wR_expected     4.685
_pd_proc_ls_prof_wR_factor       7.604
_pd_proc_number_of_points        5250
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.623
_refine_ls_R_I_factor            1.41
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            Lu2p97Ce0p03Mg0p5Al4Si0p5O12.cif
_cod_data_source_block           a
_cod_original_cell_volume        1701.546(15)
_cod_original_sg_symbol_Hall
;
-I 4bd 2c 3
;
_cod_original_sg_symbol_H-M      Ia-3d
_cod_original_formula_sum
;
Al32 Ce0.24 Lu23.76 Mg4 O96 Si4
;
_cod_database_code               7226446
_cod_database_fobs_code          7226446